Download presentation

Presentation is loading. Please wait.

1
**MECHANICAL PROPERTIES OF MATERIALS**

Stress‑Strain Relationships Hardness Effect of Temperature on Properties Fluid Properties Viscoelastic Behavior of Polymers ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

2
**Mechanical Properties in Design and Manufacturing**

Mechanical properties determine a material’s behavior when subjected to mechanical stresses Properties include elastic modulus, ductility, hardness, and various measures of strength Dilemma: mechanical properties that are desirable to the designer, such as high strength, usually make manufacturing more difficult ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

3
**Stress‑Strain Relationships**

Three types of static stresses to which materials can be subjected: Tensile - stretching the material Compressive - squeezing the material Shear - causing adjacent portions of the material to slide against each other Stress‑strain curve - basic relationship that describes mechanical properties for all three types ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

4
Tensile Test Most common test for studying stress‑strain relationship, especially metals In the test, a force pulls the material, elongating it and reducing its diameter (left) Tensile force applied and (right) resulting elongation of material ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

5
Tensile Test Specimen ASTM (American Society for Testing and Materials) specifies preparation of test specimen ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

6
**Tensile Test Setup Tensile testing machine**

©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

7
Tensile Test Sequence (1) no load; (2) uniform elongation and area reduction; (3) maximum load; (4) necking; (5) fracture; (6) putting pieces back together to measure final length ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

8
**Engineering Stress Defined as force divided by original area:**

where e = engineering stress, F = applied force, and Ao = original area of test specimen ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

9
**Engineering Strain Defined at any point in the test as**

where e = engineering strain; L = length at any point during elongation; and Lo = original gage length ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

10
**Typical Engineering Stress-Strain Plot**

Typical engineering stress‑strain plot in a tensile test of a metal Two regions: Elastic region Plastic region ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

11
**Elastic Region in Stress‑Strain Curve**

Relationship between stress and strain is linear Hooke's Law: e = E e where E = modulus of elasticity Material returns to its original length when stress is removed E is a measure of the inherent stiffness of a material Its value differs for different materials ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

12
**Yield Point in Stress‑Strain Curve**

As stress increases, a point in the linear relationship is finally reached when the material begins to yield Yield point Y can be identified by the change in slope at the upper end of the linear region Y = a strength property Other names for yield point: Yield strength Yield stress Elastic limit ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

13
**Plastic Region in Stress‑Strain Curve**

Yield point marks the beginning of plastic deformation The stress-strain relationship is no longer guided by Hooke's Law As load is increased beyond Y, elongation proceeds at a much faster rate than before, causing the slope of the curve to change dramatically ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

14
**Tensile Strength in Stress‑Strain Curve**

Elongation is accompanied by a uniform reduction in cross‑sectional area, consistent with maintaining constant volume Finally, the applied load F reaches a maximum value, and engineering stress at this point is called the tensile strength TS (a.k.a. ultimate tensile strength) TS = ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

15
**Ductility in Tensile Test**

Ability of a material to plastically strain without fracture Ductility measure = elongation EL where EL = elongation; Lf = specimen length at fracture; and Lo = original specimen length Lf is measured as the distance between gage marks after two pieces of specimen are put back together ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

16
True Stress Stress value obtained by dividing the instantaneous area into applied load where = true stress; F = force; and A = actual (instantaneous) area resisting the load ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

17
True Strain Provides a more realistic assessment of "instantaneous" elongation per unit length ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

18
**True Stress-Strain Curve**

True stress‑strain curve for previous engineering stress‑strain plot ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

19
**Strain Hardening in Stress-Strain Curve**

Note that true stress increases continuously in the plastic region until necking In the engineering stress‑strain curve, the significance of this was lost because stress was based on the original area value It means that the metal is becoming stronger as strain increases This is the property called strain hardening ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

20
**True Stress-Strain in Log-Log Plot**

True stress‑strain curve plotted on log‑log scale. ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

21
Flow Curve Because it is a straight line in a log-log plot, the relationship between true stress and true strain in the plastic region is where K = strength coefficient; and n = strain hardening exponent ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

22
**Categories of Stress-Strain Relationship: Perfectly Elastic**

Behavior is defined completely by modulus of elasticity E Fractures rather than yielding to plastic flow Brittle materials: ceramics, many cast irons, and thermosetting polymers ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

23
**Stress-Strain Relationships: Elastic and Perfectly Plastic**

Stiffness defined by E Once Y reached, deforms plastically at same stress level Flow curve: K = Y, n = 0 Metals behave like this when heated to sufficiently high temperatures (above recrystallization) ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

24
**Stress-Strain Relationships: Elastic and Strain Hardening**

Hooke's Law in elastic region, yields at Y Flow curve: K > Y, n > 0 Most ductile metals behave this way when cold worked ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

25
Compression Test Applies a load that squeezes the ends of a cylindrical specimen between two platens Compression force applied to test piece and resulting change in height and diameter ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

26
**Compression Test Setup**

©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

27
**Engineering Stress in Compression**

As the specimen is compressed, its height is reduced and cross‑sectional area is increased e = - where Ao = original area of the specimen ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

28
**Engineering Strain in Compression**

Engineering strain is defined Since height is reduced during compression, value of e is negative (the negative sign is usually ignored when expressing compression strain) ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

29
**Stress-Strain Curve in Compression**

Shape of plastic region is different from tensile test because cross section increases Calculated value of engineering stress is higher ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

30
**Tensile Test vs. Compression Test**

Although differences exist between engineering stress‑strain curves in tension and compression, the true stress‑strain relationships are nearly identical Since tensile test results are more common, flow curve values (K and n) from tensile test data can be applied to compression operations When using tensile K and n data for compression, ignore necking, which is a phenomenon peculiar to strain induced by tensile stresses ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

31
**Testing of Brittle Materials**

Hard brittle materials (e.g., ceramics) possess elasticity but little or no plasticity Conventional tensile test cannot be easily applied Often tested by a bending test (also called flexure test) Specimen of rectangular cross‑section is positioned between two supports, and a load is applied at its center ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

32
Bending Test Bending of a rectangular cross section results in both tensile and compressive stresses in the material: (left) initial loading; (right) highly stressed and strained specimen ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

33
**Testing of Brittle Materials**

Brittle materials do not flex They deform elastically until fracture Failure occurs because tensile strength of outer fibers of specimen are exceeded Failure type: cleavage - common with ceramics and metals at low temperatures, in which separation rather than slip occurs along certain crystallographic planes ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

34
**Transverse Rupture Strength**

The strength value derived from the bending test: where TRS = transverse rupture strength; F = applied load at fracture; L = length of specimen between supports; and b and t are dimensions of cross section ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

35
Shear Properties Application of stresses in opposite directions on either side of a thin element: (a) shear stress and (b) shear strain ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

36
**Shear Stress and Strain**

Shear stress defined as where F = applied force; and A = area over which deflection occurs. Shear strain defined as where = deflection element; and b = distance over which deflection occurs ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

37
**Torsion Stress-Strain Curve**

Typical shear stress‑strain curve from a torsion test ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

38
**Shear Elastic Stress‑Strain Relationship**

In the elastic region, the relationship is defined as where G = shear modulus, or shear modulus of elasticity For most materials, G 0.4E, where E = elastic modulus ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

39
**Shear Plastic Stress‑Strain Relationship**

Relationship similar to flow curve for a tensile test Shear stress at fracture = shear strength S Shear strength can be estimated from tensile strength: S 0.7(TS) Since cross‑sectional area of test specimen in torsion test does not change as in tensile and compression, engineering stress‑strain curve for shear true stress‑strain curve ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

40
**Hardness Resistance to permanent indentation**

Good hardness generally means material is resistant to scratching and wear Most tooling used in manufacturing must be hard for scratch and wear resistance ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

41
Hardness Tests Commonly used for assessing material properties because they are quick and convenient Variety of testing methods are appropriate due to differences in hardness among different materials Most well‑known hardness tests are Brinell and Rockwell Other test methods are also available, such as Vickers, Knoop, Scleroscope, and durometer ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

42
Brinell Hardness Test Widely used for testing metals and nonmetals of low to medium hardness A hard ball is pressed into specimen surface with a load of 500, 1500, or 3000 kg ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

43
**Brinell Hardness Number**

Load divided into indentation area = Brinell Hardness Number (BHN) where HB = Brinell Hardness Number (BHN), F = indentation load, kg; Db = diameter of ball, mm, and Di = diameter of indentation, mm ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

44
**Rockwell Hardness Test**

Another widely used test A cone shaped indenter is pressed into specimen using a minor load of 10 kg, thus seating indenter in material Then, a major load of 150 kg is applied, causing indenter to penetrate beyond its initial position Additional penetration distance d is converted into a Rockwell hardness reading by the testing machine ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

45
**Rockwell Hardness Test**

(1) initial minor load and (2) major load. ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

46
**Effect of Temperature on Properties**

General effect of temperature on strength and ductility ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

47
Hot Hardness Ability of a material to retain hardness at elevated temperatures Typical hardness as a function of temperature for several materials ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

48
**Recrystallization in Metals**

Most metals strain harden at room temperature according to the flow curve (n > 0) But if heated to sufficiently high temperature and deformed, strain hardening does not occur Instead, new grains form that are free of strain The metal has recrystallized The metal behaves as a perfectly plastic material; that is, n = 0 ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

49
**Recrystallization Temperature**

Recrystallization temperature of a given metal = about one‑half its melting point (0.5 Tm) as measured on an absolute temperature scale Recrystallization takes time The recrystallization temperature is specified as the temperature at which new grains are formed in about one hour ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

50
**Recrystallization and Manufacturing**

Recrystallization can be exploited in manufacturing Heating a metal to its recrystallization temperature prior to deformation allows a greater amount of straining Lower forces and power are required to perform the process Forming a metal at temperatures above its recrystallization temperature is called hot working ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

51
**Fluid Properties and Manufacturing**

Fluids flow - they take the shape of the container that holds them Many manufacturing processes are accomplished on materials converted from solid to liquid by heating Called solidification processes Examples: Metals are cast in molten state Glass is formed in a heated and fluid state Polymers are almost always shaped as fluids ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

52
Viscosity in Fluids Viscosity is the resistance to flow that is characteristic of a given fluid Flow is a defining characteristic of fluids, but the tendency to flow varies for different fluids Viscosity is a measure of the internal friction when velocity gradients are present in the fluid The more viscous the fluid, the higher the internal friction and the greater the resistance to flow Reciprocal of viscosity is fluidity ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

53
Viscosity Viscosity can be defined using two parallel plates separated by a distance d and a fluid fills the space between the two plates ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

54
Shear Stress Shear stress is the frictional force exerted by the fluid per unit area Motion of the upper plate is resisted by this frictional force resulting from the shear viscosity of the fluid This force F can be reduced to a shear stress by dividing by plate area A ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

55
Shear Rate Shear stress is related to shear rate, defined as the change in velocity dv relative to dy where = shear rate, 1/s; dv = change in velocity, m/s; and dy = change in distance y, m Shear rate = velocity gradient perpendicular to flow direction ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

56
Shear Viscosity Shear viscosity is the fluid property that defines the relationship between F/A and dv/dy; that is, or where = a constant of proportionality called the coefficient of viscosity, Pa-s For Newtonian fluids, viscosity is a constant For non-Newtonian fluids, it is not ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

57
**Coefficient of Viscosity**

Rearranging, coefficient of viscosity can be expressed: Viscosity of a fluid is the ratio of shear stress to shear rate during flow ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

58
**Flow Rate and Viscosity of Polymers**

Viscosity of a thermoplastic polymer melt is not constant It is affected by flow rate Its behavior is non-Newtonian A fluid that exhibits this decreasing viscosity with increasing shear rate is called pseudoplastic This behavior complicates analysis of polymer shaping processes such as injection molding ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

59
**Newtonian versus Pseudoplastic Fluids**

Viscous behaviors of Newtonian and pseudoplastic fluids Polymer melts exhibit pseudoplastic behavior For comparison, the behavior of a plastic solid material is shown. ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

60
**Viscoelastic Behavior**

Material property that determines the strain that the material experiences when subjected to combinations of stress and temperature over time Combination of viscosity and elasticity ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

61
**Elastic Behavior vs. Viscoelastic Behavior**

(a) Response of elastic material; and (b) response of a viscoelastic material Material in (b) takes a strain that depends on time and temperature ©2010 John Wiley & Sons, Inc. M P Groover, Principles of Modern Manufacturing 4/e SI Version

Similar presentations

Presentation is loading. Please wait....

OK

Material testing Lesson 2.

Material testing Lesson 2.

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Maths ppt on surface area and volume Ppt on various types of web browsers and their comparative features Ppt on bmc remedy service Ppt on my school days Ppt on narendra modi Convert pdf to ppt online download Introduction to liquid crystal display ppt online Ppt on power system operation and control Ppt on p&g company Quantum dot display ppt online